Series of Novel 3D Heterometallic Frameworks Based on the Co(II) Coordination Chains and Ln(III) Coordination Layers
Liao, Sheng-Yun; Gu, Wen; Yang, Lin-Yan; Li, Tian-Hao; Tian, Jin-Lei; Wang, Li; Zhang, Ming; Liu, Xin; Crystal Growth & Design 12 (2012) 3927–; doi:10.1021/cg300326e

data_4506443
_publ_section_title
;
 Series of Novel 3D Heterometallic Frameworks Based on the Co(II)
 Coordination Chains and Ln(III) Coordination Layers
;
_journal_issue                   8
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              3927
_journal_paper_doi               10.1021/cg300326e
_journal_volume                  12
_journal_year                    2012
_chemical_formula_sum            'C40 H28 Ce2 Co N12 O20'
_chemical_formula_weight         1335.91
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                86.260(2)
_cell_angle_beta                 84.661(3)
_cell_angle_gamma                64.421(2)
_cell_formula_units_Z            1
_cell_length_a                   9.1359(7)
_cell_length_b                   10.7085(8)
_cell_length_c                   12.7553(9)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      54.96632
_cell_measurement_theta_min      6.096354
_cell_volume                     1120.25(14)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0304
_diffrn_reflns_av_sigmaI/netI    0.0373
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            11353
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         3.07
_exptl_absorpt_coefficient_mu    2.461
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.3795
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.980
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             655
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.26
_exptl_crystal_size_min          0.24
_refine_diff_density_max         0.793
_refine_diff_density_min         -1.978
_refine_diff_density_rms         0.126
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.227
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     352
_refine_ls_number_reflns         5102
_refine_ls_number_restraints     8
_refine_ls_restrained_S_all      1.226
_refine_ls_R_factor_all          0.0324
_refine_ls_R_factor_gt           0.0311
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0221P)^2^+2.4447P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0761
_refine_ls_wR_factor_ref         0.0767
_reflns_number_gt                4993
_reflns_number_total             5102
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg300326e_si_003.cif
_cod_data_source_block           co-ce
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4506443